Revista Romn de Materiale / Romanian Journal of Materials 2016, 46 (1), 63 69 63
FILME SUBIRI TRANSPARENTE CONDUCTOARE CODOPATE CU Al I In DEPUSE PRIN PULVERIZARE CU PIROLIZ
TRANSPARENT CONDUCTING Al AND In CODOPED THIN FILM DEPOSITED BY SPRAY PYROLYSIS
A. HADRI1, B. FARES1, A. AMARI1, M. TAIBI2 ,A. MZERD1
1University Mohammed V- Rabat, Faculty of Sciences, Physics Department, LPM, B.P. 1014, Agdal-Rabat, Morocco. 2University of Mohammed V, Ecole Normale Superieure,LPCMIN, Rabat-Morocco
Transparent conducting Al-In codoped ZnO thin films were successfully synthesized onto glass substrates by spray pyrolysis technique. The influence of doping and codoping on the structural, optical and electrical properties was investigated. X-ray diffraction results showed that the samples have the hexagonal Wrtzite structure with a preferred orientation toward the c-axis. No peaks belonging to In and Al or their oxides was observed in the limit of XRD technique detection. EDS analysis confirmed the presence of In and Al elements in ZnO thin films. The atomic percentage of In and Al elements was nearly equal to their nominal stoichiometry. The surface morphology of the codoped films showed well-defined hexagonal grains. Examination through transmission electron microscopy depicted that these films consists of an agglomeration of small grains with hexagonal shape. A high transmittance above 75% and electrical resistivity around 310-2 .cm were reached after annealing.
Keywords: Spray pyrolysis, Hall Effect, ZnO, aluminum-indium codoped ZnO. 1. Introduction
Among various transparent conducting oxides (TCO), zinc oxide (ZnO) has been received more and more attention. It holds an important position in the field of material science due to its wide band gap, large exciton binding energy (60 meV) and high stability in hydrogen plasma [1-4]. These unique properties make ZnO extensively used in a wide range of applications such as transistors , solar cells and sensors [6-7]. Recently, several physical and chemical methods have been employed to prepare ZnO thin films such as magnetron sputtering , pulsed laser deposition , chemical vapor deposition , spray pyrolysis , sol-gel . Generally, physical techniques are commonly used; however the cost is relatively high. In the present investigation we will focus on the spray pyrolysis technique due to its cost effectiveness as it does not require sophisticated vacuum apparatus and well adapted for mass fabrication.
The electrical conductivity of undoped ZnO is relatively low, which cannot meet the demands of several application fields. To improve electrical, optical and other properties of ZnO, It is practical to dope ZnO with group III elements [13-15]. In single doped ZnO, Al doped ZnO (AZO) have attracted most of the researchers attention due to its numerous advantages in terms of conductivity and chemical stability [16-18], while others choose In as
dopant (IZO) due to its lower reactivity and greater resistivity to oxidation [19-20]. Furthermore, studies emphasized that codoping with low concentration in ZnO films can optimize their physical properties. For example, Al-V codoped ZnO and Al-Y codoped ZnO thin films have showed an improved thermal stability and electrical conductivity, respectively [21-22]. Therefore, it appears that Al and In codoped ZnO (IAZO) can be attractive.
In this paper, undoped ZnO,IZO and IAZO thin film were synthesized on glass substrates by spray pyrolysis method and the structure, electrical and optical properties of these films were studied and discussed.
2. Experimental details
Undoped ZnO, IZO and IAZO thin films were successfully synthesized on glass substrates by spray pyrolysis technique using different Al content. A homogenous solution were prepared by dissolving zinc chloride ZnCl2, Indium Chloride InCl3 and aluminum nitrate nona-hydrate (Al(NO3)3,9H2O) in 200 mL of distilled water in order to prepare the starting solution with a concentration of 0.05M. Undoped ZnO and IZO were used as a reference samples. The Al content was varied at 0 at.%, 1 at.% and 2 at.%, while In content was fixed at 3 at.%, and were named IZO3, IAZO1 and IAZO2 respectively. The content of Al and In in the starting solution is referred here as the
Autor corespondent/Corresponding author, E-mail: [email protected]
64 A.Hadri, B. Fares, A. Amari, M. Taibi, A. Mzerd / Transparent conducting Al and In codoped thin film deposited by spray pyrolysis
atomic percentage with respect to Zn. The detailed description of experimental procedure has been given elsewhere . The as deposited IZO3, IAZO1 and IAZO2 were annealed in tubular furnace at 350 C for 2h in argon atmosphere.
The deposited films were characterized in order to study their chemical and physical properties. X-ray diffraction (XRD, Siemens D 5000) was carried out, using Cu-k radiation, =1.5405, to analyze the crystallite size and growth orientation of the as-deposited films. The In/metal and Al/metal composition of the films on glass substrates were investigated by energy dispersive spectroscopy (EDS). The surface morphology and topography were examined by Scanning Electron Microscopy (SEM, FEI Quanta 200) and Atomic Force Microscopy (AFM), operating in tapping mode. Transmission electron microscope (TEM) micrographs were obtained using Topcon 002b. Electrical properties of the films have been performed by Ecopia HMS 3000 Hall effect measurements system using the four probes Van der Pauw configuration. The measurements have been done at room temperature and the ohmic behavior of the contacts has been confirmed prior to Hall measurements. The Hall measurements have been repeated several times for each sample to confirm the consistency of our results. The optical transmittance spectra were obtained using UV- visible spectrophotometer (PerKilmer Lambda 900) and taking into account the glass in the reference beam.
3. Results and discussion 3.1. Structure and surface morphology
To investigate the effect of doping and codoping on the microstructure of the elaborated thin films, XRD analysis was performed. Figure 1 illustrates the XRD patterns of undoped ZnO, IZO and IAZO thin films.
Fig. 1 - X-ray diffraction spectra of the deposited thin films.
As seen from this figure, four diffraction peaks are observed which are related to (100), (002), (101) and (102) orientations [JCPDS-card
No 89-1397], indicating a polycrystalline structure that belonged to the ZnO wrtzite structure. The absence of other peaks even for the film deposited with highest Al content in the starting solution precludes the possibility of any extra phases related to Al or In in the films (within the sensitivity limitation of XRD). In all cases, the other peaks are lower in comparison with (002) peak suggesting that the crystalline structure of the films is mainly oriented with their c-axis perpendicular to the substrate irrespective of the doping content. Moreover, the (002) diffraction peak is the sharpest when the Al content is 1at.%, which implied that the impurities were stabilized in the IAZO1 structure system. L. Balakrishnan et al. confirmed that the high intensity of (002) peak was attributed to the improvement of stoichiometry by optimum incorporation of dopant atoms .
The texture coefficient  (TC) of the (002) plane was calculated and listed in Table1. It is seen that all the thin films have a (002) preferential orientation and that the codoped films with the lowest Al content shows the highest value. This could be attributed to the small ionic radius of aluminum compared to that of zinc and indium, which at lower concentration occupy mainly substitution sites and therefore change the growth pattern. As the Al content increases above 1%, the texture coefficient decreases which may be due to the limited solubility of Aluminum. As a consequence, the aluminum excess may occupy interstitial sites that affect the cystallinity of the films.
Structural parameters of ZnO, IZO and IAZO thin films
Samples D(nm) TC(002) () ()
ZnO 49.1 2.81 3.190 5.210
IZO3 34.6 1.96 3.202 5.230
IAZO1 28.1 3.84 3.197 5.222
IAZO2 29.7 2.96 3.198 5.223
The crystallite size of the films were
calculated from the (002) peak in the XRD profile by using Scherrers formula  (see Table 1). The significant decrease in grain size was attributed to the fact that some of the doping atoms prefer to locate in the grain boundary regions and inhibit the grain growth due to the difference of atomic radius of zinc and doping elements (In, Al).
The lattice constant ( ) and ( ) were obtained using the inter-reticular distance dhkl of the hexagonal structure and are found to be in good agreement with the usually published values of ZnO [26, 27]. Compared to the undoped ZnO film, the increase in the lattice constant observed in IZO3 thin film was attributed to the difference in
A.Hadri, B. Fares, A. Amari, M. Taibi, A. Mzerd / Filme subiri transparente conductoare codopate cu Al i In 65 depuse prin pulverizare cu piroliz
the ionic radii of zinc and indium (RZn2+=0.074 nm and RIn3+=0.08 nm). On the other hand, the lattice parameter of the codoped film exhibits two behaviors. At low aluminum cont